Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Document related concepts

Transcript

Optical Fredericks Transition in a Nematic Liquid Crystal Layer Hong Zhou, Eric P. Choate, and Hongyun Wang Abstract: One of the most fascinating aspects of liquid crystals is the Fredericks transition, which can occur when a finite sample of nematic liquid crystal is subjected to an externally applied magnetic or electric field. It is well-known that the director orientation throughout a sample of liquid crystal may be affected by a sufficiently strong magnetic or electric field. More specifically, the director alignment throughout a thin sample of nematic liquid crystal will not be influenced by the external magnetic or electric field when its magnitude is less than the critical field strength or Fredericks threshold, but will be influenced by the external field and start to adjust its orientation whenever the magnitude of the field is above the critical field strength. This change in the director alignment after the magnitude of the field increases beyond the critical field strength is called the Fredericks transition. It is exactly this important aspect of liquid crystals that provides many applications of liquid crystals for displays. In this chapter we first review the classical Fredericks transition in a liquid crystal H. Zhou (corresponding author) Department of Applied Mathematics, Naval Postgraduate School, Monterey, CA 93943, U.S.A. E.P. Choate Department of Mathematics and Statistics, Radford University, Radford, VA 24142, U.S.A. H. Wang Department of Applied Mathematics and Statistics, University of California, Santa Cruz, CA 95064, U.S.A. Hong Zhou, Eric P. Choate and Hongyun Wang layer where analytical solutions can be obtained. After this warm-up, we provide a detailed analysis in modeling electrically induced Fredericks transition. We conclude the chapter with some future perspectives. Keywords: Fredericks transition; nematic liquid crystals; continuum theory; critical threshold 1. Introduction and Overview The term "liquid crystals" was first introduced by Otto Lehmann in 1889 and it is quite self-explanatory. It describes a matter state where materials exhibit many properties of solid crystals such as anisotropy and symmetry, but flow like fluids or viscous fluids. This combination of properties makes liquid crystals absolutely unique and complex materials. There are many different types of liquid crystal phases. One of the most common phases is the nematic phase where the rod-like molecules tend to be aligned parallel to each other along some common preferred direction (“anisotropic axis”). Examples of nematic liquid crystals include p-azoxyanisole (PAA), 4-methoxybenzylidene-4’-butylaniline (MBBA) and 4-pentyl-4’-cyanobiphenyl (5CB). In a typical nematic such as PAA the molecules closely resemble rigid rods of o o o length 20 A and width 5 A (de Gennes and Prost 1993) where 1 angstrom A equals 10−10 m . The state of PAA depends on the temperature. PAA is a solid below 118o C , a nematic liquid crystal between 118o C and 135.5o C , and an isotropic liquid above 135.5o C (de Jeu 1980). The local direction of the average molecular alignment in liquid crystals is usually described by a unit vector n , called the "director". Due to the lack of polarity of liquid crystals the two vectors n and −n 2 Optical Fredericks Transition in a Liquid Crystal Layer are indistinguishable. Liquid crystals have been used in a wide variety of applications because external perturbation can cause significant changes in the macroscopic properties of the liquid crystal system. Both electric and magnetic fields can be applied to induce these changes. In fact, one of the most intensively studied phenomena in the physics of liquid crystals is the Fredericks transition which has been known for over 80 years. It refers to a transition from a uniform director configuration to a deformed director configuration of a homeotropically or planarly aligned nematic liquid crystal (NLC) layer upon application of a magnetic or electric field of sufficiently large magnitude. The behavior of a nematic liquid crystal is determined by two competing torques: (1) the elastic torque within the material that tries to align the NLC molecules along the easy direction as determined by the anchoring boundary conditions; and (2) external-field-induced torque that tends to align the NLC molecules either parallel or orthogonal to the field. A uniform director distribution occurs when only one of these torques is present. When both torques exist, there is a competition between them. Once the applied field strength exceeds a threshold value, the uniform NLC orientation will deform and the Fredericks transition takes place. The description of how the director is aligned on the boundary surfaces is called anchoring. The main types of anchoring include strong, weak and conical anchoring. Strong anchoring occurs when the surface energy is sufficiently large and the director orientation on the boundary of the sample can be considered simply fixed in a preferred orientation determined by an alignment technique. In the case of weak 3 Hong Zhou, Eric P. Choate and Hongyun Wang anchoring, the director alignment on the boundary is no longer rigidly fixed to the surface and it is allowed to vary. Conical anchoring refers to the situation where the director at a boundary makes a fixed angle with the tangent plane of the boundary. Strong anchoring conditions are commonly used due to their simplicity. There are several kinds of strong anchoring boundary conditions. For the planar alignment, the molecules lie parallel to the cell surface. It can be obtained by either rubbing the alignment layer (usually a polyimide thin film) or by UV photo-alignment. For the homeotropic alignment, the director is perpendicular to the cell surface. It is obtained by means of detergents or by applying a surfactant to the alignment surface. It is also possible to obtain any pretilt angle by evaporating silicon dioxide at different angles of incidence. Other alignment techniques, such as micron rubbing by microsphere, micro-contact printing, ion beam bombardment, are available as well (Yilmaz et al. 2008). The Fredericks transition plays a fundamental role in the operation of many liquid crystal displays because the director orientation can be controlled easily by an external magnetic or electric field. One striking feature is that the magnitude of the Fredericks threshold voltage is essential to the operation of many liquid-crystal devices. If the Fredericks threshold voltage could be reduced reliably, this would make it possible for the manufacture of very low-power liquid crystal displays and other liquid-crystalline devices. The Fredericks transition can also be employed to achieve tunable all-optical switching and diode operation in the photonic devices (Miroshnichenko et al. 2006). 4 Optical Fredericks Transition in a Liquid Crystal Layer There have been many studies on the Fredericks transition. For example, experimental observations include the first observation of the optical-field-induced Fredericks transition in the nematic liquid crystal 5CB (Durbin et al. 1981), nonlinear light amplification in MBBA above the Fredericks transition by a magnetic field (Khoo and Zhuang 1980). A quantitative theory to describe the reorientation of the director of a nematic liquid crystal induced by the field of a light wave was developed by Zel’dovich et al. using the geometrical optics approximation (Zel’dovich and Tabiryan 1980; Zel’dovich, Tabiryan and Chilingaryan 1981). They calculated the solution for the spatial distribution of the director direction for intensities above and below threshold. They noted that a Fredericks transition induced by light fields in an NLC with a positive dielectric anisotropy ( ε a > 0 ) can occur only when the light wave is normally incident on an NLC cell with homeotropic orientation. When an ordinary light wave is normally incident on an NLC cell with planar orientation, Fredericks transition will not occur. They also predicted that near the threshold the maximum angle of deviation of the director from the unperturbed direction is proportional to the square root of the excess of the intensity above the threshold intensity and that for certain nematic liquid crystals the Fredericks transition in a light field is accompanied by hysteresis in broad beams, which they believed has no analog in the case of static fields. In fact, in 1974 Deuling and Helfrich (Deuling and Helfrich 1974) had shown that a homeotropic nematic layer with negative dielectric (or conductive) anisotropy enclosed between two metallized glass plates undergoes a Fredericks transition. In 1981 Durbin et al. (Durbin et al. 1981) expressed the total electromagnetic energy 5 Hong Zhou, Eric P. Choate and Hongyun Wang density as the ratio of the magnitude of the Poynting vector to the ray velocity and then used the infinite-plane-wave approximation in which the time average of the magnitude of the Poynting vector of the optical field was assumed to be a constant throughout the medium. Minimization of the free energy led to the Euler equation. The solution of the Euler equation with proper boundary conditions gave the average molecular reorientation of the liquid crystal. Their theoretical predictions were in quantitative agreement with their experimental results. These earlier theoretical studies only took the large anisotropies of nematic liquid crystals into account but they lack the ability to properly describe the associated nonlinear effects. The ground-breaking treatment of the optically induced Fredericks transition was given by Ong (Ong 1983). In this classical work Ong provided a detailed study which includes the interaction between the optical field and the NLC. An Euler equation, which is consistent with Maxwell’s equations, is derived for describing the optically induced spatial reorientation of the director of a homeotropically oriented nematic liquid crystal for the case of normal incidence. The solution of the Euler equation describes the deformation angle of the NLC. By examining the maximum deformation angle near the threshold, Ong obtained the threshold intensity and the criterion for the physical parameters that indicate whether the Fredericks transition is first order or second order at the threshold. In contrast to Durbin’s assumption, Ong showed that the time average of the magnitude of the Poynting vector is not a constant, but the time average of the z-component of the Poynting vector is a constant, which is consistent with the geometrical optics approximation (Zel’dovich and Tabiryan 1980; 6 Optical Fredericks Transition in a Liquid Crystal Layer Zel’dovich, Tabiryan and Chilingaryan 1981). In 1995 Sugimura et al. (Sugimura, Luckhurst and Ou-Yang 1995) generalized the Rapini-Papoular formula (Rapini and Papoular 1969) for the anchoring energy and provided rigorous expressions for the threshold and saturation fields for a field-controlled twisted chiral nematic slab with weak boundary coupling. Self, Please and Sluckin (Self, Please and Sluckin 2002) considered the situation where the electromagnetic field interacts with the liquid crystal deformation. Assuming strong anchoring at solid surfaces and a one-dimensional distortion, they identified three dimensionless parameters, which are related to the elastic anisotropy of the liquid crystal, the anisotropy of the electrical permittivity of the liquid crystal, and the applied voltage, respectively. They applied systematic asymptotic methods to determine approximate solutions in five various regimes defined by physically relevant limiting cases of the parameters. Shi (Shi 2002) summarized the main results in his two papers (Shi and Yue 2000, Yang, Shi and Liang 2000) to give the exact criteria for the first order Fredericks transition to occur in magnetically, electrically or optically driven liquid crystal cells. All these criteria are in terms of the material parameters, cell geometrical parameters and surface anchoring parameters where the anchoring strengths at the surfaces are described by the Rapini- Papoular surface anchoring energy. It was noted that the first order magnetic or electrical Fredericks transition occurs at surface anchoring conditions that current technology is not mature enough to achieve. The first order transition cannot occur for a rigid anchoring condition and this explains why first order transitions in the magnetic and electrical cases are so difficult to observe. However, the first order 7 Hong Zhou, Eric P. Choate and Hongyun Wang transition can be easily realized for a three-dimensional Fredericks transition, as in a twist liquid crystal cell. Colloidal suspensions – dispersions of small solid particles in a host liquid consisting of small molecules -- in nematic liquid crystals can also undergo Fredericks transition. For a general review on the physics of colloidal dispersions in nematic liquid crystals, see the article by Stark (Stark 2001). Ferronematics is the name for suspensions of monodomain ferro or ferromagnetic particles in nematic liquid crystals. Dispersed ferromagnetic particles greatly enhance the magnetic properties of the liquid crystals. In 2003 Bena and Petrescu (Bena and Petrescu 2003) considered an infinite flat layer of ferronematics (FN) between two identical substrates to study the magnetic field-induced Fredericks transition in a homeotropically aligned FN with weak anchoring molecules to the walls. They have found a correction to the Burylov-Raikher expression (Burylov and Raikher 1993) for the magnetic threshold field, together with an expression for the saturation magnetic field as a function of material parameters and anchoring conditions. The saturation transition does not occur in the case of rigid anchoring molecules to the cell walls. In 2009 they extended their work to analyze the influence of anchoring conditions on the Fredericks transition in ferronematics subjected to a superposed magnetic static field and an optical field (Petrescu and Bena 2009). Using the Rapini-Papoular expression (Rapini and Papoular 1969) for the anchoring energy and the Euler-Lagrange analytical method, they obtained a correlation between the threshold intensities of the magnetic and the laser fields, the anchoring strength, the material and device parameters. They found 8 Optical Fredericks Transition in a Liquid Crystal Layer that the fields needed for the transition are smaller than those in the rigid anchoring case. Another system analogous to ferronematics involves ferroelectric rather than ferromagnetic colloidal particles. The colloidal particles are extremely small and at low concentrations these submicron colloids macroscopically appear similar to a pure liquid crystal with no evidence of dissolved particles. These dilute suspensions are stable because the nanoparticles do not significantly perturb the director field in the liquid crystals, and interaction between the particles is weak. In these colloidal suspensions the dielectric response is strongly enhanced and the values of the effective dielectric functions are higher than those of the analogous pure liquid crystals. Such systems were first fabricated by Reznikov et al. (Reznikov et al. 2003) using particles of the ferroelectric thiohypodiphosphate ( Sn2 P2 S6 ) for the suspension and have been the subject of many researches (e.g. Li et al. 2006 and Shelestiuk, Reshetnyak and Sluckin 2011). Shelestiuk et al. (Shelestiuk, Reshetnyak and Sluckin 2011) explored the Fredericks transition in ferroelectric liquid-crystal nanosuspensions. Their study suggested that doping a nematic liquid crystal with ferroelectric particles can significantly decrease the electric Fredericks threshold field. A computational approach to the optical Fredericks transition in a homeotropic nematic liquid crystal cell has been provided by Ilyina, Cox and Sluckin (Ilyina, Cox and Sluckin 2006). They combined the popular finite difference time domain (FDTD) method to solve the Maxwell’s equations with a relaxation algorithm to solve the Ginzburg-Landau equations for the liquid crystal director. 9 Hong Zhou, Eric P. Choate and Hongyun Wang As one can see, it is impossible for us to provide a comprehensive list of all relevant publications on the Fredericks transition in liquid crystals. For more details on the theory and application of liquid crystals, please refer to the books by de Gennes and Prost (de Gennes and Prost 1993), Chandrasekhar (Chandrasekhar 1992), Khoo (Khoo 1995), Virga (Virga 1994) and Stewart (Stewart 2004). 2. The Classical Fredericks Transitions in a Nematic Liquid Crystal Cell In general, the classical Fredericks transition in nematics can be fairly well-explained using continuum theory of nematic liquid crystals developed by Frank, Ericksen and Leslie. Before we present a detailed analysis on the optical Fredericks transition, which couples the interaction between the applied electromagnetic field of a light wave and the orientation of liquid crystals, we would like to briefly review the classical results (de Gennes and Prost 1993, Virga 1994, Stewart 2004). Many of our ideas here are borrowed from Stewart (Stewart 2004). Conventional analytic study of this problem normally considers an electromagnetic field in which the magnetic component is dominant. Generally the effect of the nematic orientation does not affect the magnetic field, and so the electromagnetic field structure decouples from the orientation and the electric field components can be ignored. To get started, let us consider a nematic liquid crystal sample confined between two parallel glass plates at 𝑧 = 0 and at 𝑧 = 𝐿. We assume strong anchoring and impose the same director at each plate. We also assume the anchoring is uniform in the x- and y-directions so that the orientation is a function of z only. 10 Optical Fredericks Transition in a Liquid Crystal Layer We will consider three common geometries concerning the relationship between the anchoring conditions and imposed magnetic field: splay, bend, and twist. For the splay geometry, the director is parallel to the bounding plates where n( z ) = (1, 0, 0 ) is the uniform equilibrium solution. In this case, the natural choice for the magnetic field to apply in order to observe the Fredericks transition is H H= = ( 0, 0,1) , H H . Assuming that the director attempts to reorient itself to be parallel to the magnetic field and any reorientation of the director only depends on z, we seek solutions for the director of the form n = ( cos φ ( z ) , 0,sin φ ( z ) ) , where φ ( z ) is called the director angle. The bend geometry reverses these roles with the director anchored perpendicularly to the plates while the magnetic field is parallel to the plates. We set the magnetic field H = H (1, 0, 0 ) and seek solutions of the form n = ( sin φ ( z ) , 0, cos φ ( z ) ) . Figure 1 illustrates these three geometries. We begin by focusing on the twist geometry, in which both the initial director alignment and the magnetic field are both parallel to the glass plates but are mutually orthogonal to each other. We impose a magnetic field of the form H = H ( 0,1, 0 ) and search for directors of the form n = ( cos φ ( z ) ,sin φ ( z ) , 0 ) . The analysis is easier in the twist geometry, and we present a detailed derivation of its solution. Afterwards, we present the splay and bend geometries, which are very similar to each other and reduce to a form like the twist geometry under a simplifying assumption. For boundary conditions in all three geometries, we use 11 Hong Zhou, Eric P. Choate and Hongyun Wang φ= ( 0 ) φ= ( L) 0 (1) so that all three have the uniform solution φ ( z ) = 0 for all 0 ≤ 𝑧 ≤ 𝐿. Below the critical field strength 𝐻𝑐 of the Fredericks transition, this uniform solution is stable, but above the critical value, a stable nonuniform solution appears. To find the stable solution, we must minimize the free energy of the system, which balances contributions from elastic and magnetic parts. The Frank elastic free energy density for nematics is given by 1 2 2 2 (2) K1 ( ∇ ⋅ n ) + K 2 ( n ⋅∇ × n ) + K 3 ( n × ∇ × n ) 2 where the Frank elasticity constants K1 , K 2 , and K 3 represent the splay, twist, and bend = f Frank moduli, respectively (Virga 1994). The elastic constants depend on temperature and are commonly of the order 10−7 to 10−6 dyn with K 3 often being two or three times larger than K1 and K 2 . For example, for PAA, at 120°C the constants are K= 5.0 ×10−7 dyn, 1 K= 3.8 ×10−7 dyn, and = 4.5 ×10−7 dyn, K 3 10.1×10−7 dyn, and at 125°C, K= 2 1 9.5 ×10−7 dyn. 2.9 ×10−7 dyn, and K= K= 2 3 For analytical purposes, it is often common to use the simplifying single-constant assumption with K= K= K= K all . Under this assumption, the Frank elastic free 1 2 3 energy density simplifies to 1 1 K all ∇n : ∇n = K all tr(∇n ⋅ (∇n)T ) . 2 2 The free energy density contribution from the magnetic field is f Frank = (3) 12 Optical Fredericks Transition in a Liquid Crystal Layer 1 2 f magnetic = − χa (n ⋅ H ) 2 (4) where χ a is the anisotropic magnetic susceptibility in Gaussian cgs units. We will assume χ a > 0 . Therefore the total free energy density= is f f Frank + f magnetic . 2.1 Twist Geometry and Single-Constant Assumption Inserting the form of the twist geometry n = ( cos φ ( z ) ,sin φ ( z ) , 0 ) and H = H ( 0,1, 0 ) into (2) and (4), we have the total free energy density 1 1 K 2 φ ′2 − χ a H 2 sin 2 φ . 2 2 f = (5) The total energy functional of φ ( z ) is obtained by integrating the free energy density over the thickness: F [φ ] = ∫ f (φ ( z ) , φ ′ ( z ) ) dz L 0 (6) To look for functions φ ( z ) that minimize F , we consider the perturbed solution φ ( z ) + δη ( z ) where η= ( 0 ) η= ( L ) 0 , and write F [φ= ] ∂f ∂f ∫ 0 f (φ , φ ′) + δ ∂φ η + ∂φ ′ η ′ L ∂2 f ∂ 2 f 2 δ ∂2 f + 2 η2 + 2 ηη ′ + η ′ dz + O (δ 3 ) 2 ∂φ ′ ∂φ∂φ ′ 2 ∂φ 2 (7) For φ ( z ) to minimize F [φ ] , the first variation must be zero: ∫ ∂f ∂f η+ η ′dz = 0. 0 ∂φ ∂φ ′ L (8) Integration by parts using the boundary conditions η= ( 0 ) η= ( L ) 0 yields 13 Hong Zhou, Eric P. Choate and Hongyun Wang ∫ ∂f d ∂f − 0. η dz = 0 ∂φ dz ∂φ ′ L (9) Since η is arbitrary, we obtain the Euler-Lagrange equation ∂f d ∂f − = 0 ∂φ dz ∂φ ′ (10) Now, substituting (5) obtains the equilibrium equation for the director angle: K 2 φ ′′ + χ a H 2 sin 2φ =0 2 (11) This equation is of the form that has been considered by Freedericksz and Zolina (Freedericksz and Zolina 1933) and Zocher (Zocher 1933). For any value of H and the boundary conditions (1), φ ( z ) = 0 is a trivial but important solution to (11). This represents a uniform solution in which the nematic orientation is homogeneous. Its stability can be seen from the second variation in (7). In order for φ ( z ) = 0 to be a minimum, we need ∂2 f 2 ∂2 f ∂2 f 2 ′ + + η ηη η ′ dz > 0 . 2 ∫ 0 ∂φ 2 ∂φ∂φ ′ ∂φ ′2 L (12) Integrating by parts and inserting (5) yields ∫ L 0 − χ a H 2 cos 2φη 2 + K 2η ′2 dz > 0 , (13) or once we inserting φ ( z ) = 0 , ∫ L 0 − χ a H 2η 2 + K 2η ′2 dz > 0 . ∞ π jz j =1 L If we assume a representation of η ( z ) = ∑η j sin (14) , we find that we must have 14 Optical Fredericks Transition in a Liquid Crystal Layer −χa H 2 + π 2 j2 L2 K2 > 0 . (15) for each j ≥ 1 for stability. The most restrictive of these is when j = 1 . Therefore, the homogeneous solution φ ( z ) = 0 minimizes the free energy if H < H c where H c ,uniform = π L K2 χa (16) The question remains as to whether or not there are other solutions. Since the free energy density (5) has an even dependence on φ , if φ ( z ) minimizes the free energy, then −φ ( z ) also minimizes the free energy. Also, due to the boundary conditions (1), we expect nontrivial solutions to take the symmetric form φ ( z= ) φ (L − z), 0 ≤ z ≤ L (17) which implies that L φ′ = 0 . 2 From (11), if φ ′ =0 and 0 < φ < (18) π L L , then φ ′′ < 0 , and so φ must be a local 2 2 2 maximum, which we will denote as φmax . We now multiply (11) by φ ′ and integrate to get K 2 φ ′2 + χ a H 2 sin 2 φ = C . (19) The constant of integration C may be found by evaluating at z = L2 : 15 Hong Zhou, Eric P. Choate and Hongyun Wang C = K 2 φ ′2 + χ a H 2 sin 2 φ z= L 2 = χ a H 2 sin 2 φmax . (20) Thus, (19) can be written as K 2 φ ′2 = χ a H 2 sin 2 φmax − sin 2 φ . (21) Since the left side is positive, we can conclude from the right side that 0 ≤ φ ≤ φmax on the interval 0 ≤ z ≤ L with φ 2 increasing monotonically from 0 to φmax . Therefore, = K2 φ ′ χ a H sin 2 φmax − sin 2 φ . Upon integration, we can define φ ( z ) on 0 ≤ z ≤ χ a Hz = K 2 ∫ 0 L implicitly through the equation 2 dφ φ (22) sin 2 φmax − sin 2 φ , (23) once we have found the value of φmax , which we may find by first solving the implicit equation coming from (23) evaluated at z = χa H L 2 and φ = φmax : φmax L dφ = K2 ∫ . 0 2 2 2 sin φmax − sin φ We can then extend the solution to the interval (24) L ≤ z ≤ L by using the symmetry (17). 2 To aid us both in analysis and computation, we can rewrite these using elliptic functions if we first make a change of variables similar to the one used by Zocher (Zocher 1933) = sinψ sin φ cos φ = , cosψ dψ dφ . sin φmax sin φmax (25) Eq. (24) can be rewritten as 16 Optical Fredericks Transition in a Liquid Crystal Layer HL χ a = 2 K2 π dψ K ( sin φmax ) = ∫ 02 1 − sin 2 ψ sin 2 φ max (26) where K ( k ) is the complete elliptic integral of the first kind with modulus k = sin φmax . MATLAB provides a built-in function ellipke to compute complete elliptic integrals of the first and second kinds. This also allows us to see that in the limit of strong magnetic fields ( H → ∞ ), we must have φmax → π− 2 . Once φmax is found, the distorted solution φ ( z ) can be found on 0 ≤ z 1 by ≤ L 2 rewriting (23) as Hz χa K2 =∫ sin φ sin −1 sin φmax 0 dψ 1 − sin ψ sin 2 φmax 2 sin φ = Felliptic sin −1 sin φmax ,sin φmax , (27) where Felliptic (ψ , k ) is the incomplete elliptic function of the first kind with modulus k = sin φmax , which can be computed in MATLAB with the built-in function ellipticF. The solution for 1 z ≤ ≤ 1 can then be obtained via the symmetry (17). 2 L This distorted solution, however, does not exist for small values of H . To see this and find the critical threshold H c ,distorted above which the distorted solution does exist, we define the function G (ψ , φmax ) ≡ 1 1 − sin 2 ψ sin 2 φmax . (28) Note that G has the symmetry G (ψ , φmax ) = G (φmax ,ψ ) . It is straightforward to check that 17 Hong Zhou, Eric P. Choate and Hongyun Wang ∂G (ψ , φmax ) sin 2 ψ sin 2φmax . = 3/2 ∂φmax 2 (1 − sin 2 ψ sin 2 φmax ) Thus, for 0 < φmax < π 2 and 0 < ψ < π 2 (29) , ∂G (ψ , φmax ) > 0. ∂φmax (30) Consequently, G (ψ , φmax ) is a monotonically increasing function of φmax for 0 < φmax < π 2 . Furthermore, note that = lim + G (ψ , φmax ) φmax →0 1 = lim + 1. φmax →0 1 − sin 2 ψ sin 2 φmax (31) Taking the limit φmax → 0+ on both sides of (26), we find that the critical field strength H c ,distorted obeys H c ,distorted L χa 2 K2 = π 2 . (32) Therefore, we find the same critical value as H c ,uniform from (16), and so we have only one critical value Hc = π L K2 χa (33) such that the uniform solution φ ( z ) = 0 is the only solution and is stable if H < H c , but for H > H c , the uniform solution is unstable and the distorted solution given by (26) and (27) exists. Also, when H > H c , we can show that the distorted solution given by (26) and (27) is energetically favorable to the uniform solution φ ( z ) = 0 by showing that the difference in the free energies of the two solutions 18 Optical Fredericks Transition in a Liquid Crystal Layer ∆F= F [φ ] − F [0] (34) is negative. From the energy expression (6) and using (21), we obtain 1 L K 2 φ ′2 − χ a H 2 sin 2 φ dz ∫ 0 2 L 1 = χ a H 2 ∫ sin 2 φmax − 2sin 2 φ dz 0 2 L L 1 2 2 =χ a H ∫ sin 2 φmax − 2sin 2 φ dz + ∫ L sin 2 φmax − 2sin 2 φ dz 0 2 2 = ∆F (35) For the second integral, we make the change of variables z= L − z so that ∫ L L 2 2 sin 2 φmax − 2sin= φ dz L 2 0 ∫ 0 L 2 sin 2 φmax − 2sin 2 φ ( L − z ) ( −dz ) (36) L 2 0 = ∫ sin φmax − 2sin φ ( z ) dz = ∫ sin φmax − 2sin φ ( z ) dz 2 2 2 2 where the symmetry condition (17) is employed. Thus, L = ∆F χ a H 2 ∫ 2 sin 2 φmax − 2sin 2 φ dz 0 = χa H 2 ∫ = φmax 0 χa H ∫ (sin 2 φmax − 2sin 2 φ ) φmax 0 ( sin 2 dz dφ dφ φmax − 2sin 2 φ ) (37) K2 sin φmax − sin φ 2 where we have differentiated (23) to get the expression of 2 dφ dz . Using the substitution dφ (25), we can rewrite this as 19 Hong Zhou, Eric P. Choate and Hongyun Wang π ∆F =χ a K 2 H sin 2 φmax ∫ 2 0 cos 2ψ 1 − sin 2 φmax sin 2 ψ dψ π = χ a K 2 H sin 2 φmax ∫ 2 cos 2ψ G (ψ , φmax ) dψ 0 = − (38) π ∂G (ψ , φmax ) 1 χ a K 2 H sin 2 φmax ∫ 2 sin 2ψ dψ 0 ∂ψ 2 where we have again used (28) and integrated by parts in the last step. Thus, we use (30) and the fact that sin 2ψ > 0 on 0 < ψ < π 2 to conclude that ∆F < 0 for H > H c . Therefore, the distorted solution is indeed energetically preferred over the unstable uniform solution, which verifies that the Fredericks transition does occur in the twist geometry and that H c ,twist = π L K2 χa (39) is the critical threshold. Under the single-constant approximation K= K= K= K all , the free energy 1 2 3 density takes the same form (5) except that K 2 is replaced with K all . Therefore all the above analysis can be repeated so that the critical threshold is Hc = π L K all χa . (40) When H < H c the uniform solution φ ( z ) = 0 is the only stable solution, but for H > H c , the stable solution is the distorted solution given by 20 Optical Fredericks Transition in a Liquid Crystal Layer H 2 = K ( sin φmax ) , Hc π sin φ 1 Hz = Felliptic sin −1 Hc L π sin φmax ,sin φmax , (41) (42) where K and Felliptic are the complete and incomplete elliptic functions of the first kind, respectively. Figure 2 illustrates the distorted solution φ ( z ) from (41) and (42) for various values of the dimensionless magnetic field strength H / H c . As H / H c increases, the values of φ ( z ) in the interior also increase. The transition that we have so far described analytically can be illustrated by the bifurcation diagram of Figure 3, where the solid line represents the stable solution and the dashed line represents the unstable one. For H ≤ H c , the trivial solution φmax= φ= 0 is the only solution of the equilibrium equation, and it is necessarily stable. For H > H c , the trivial solution becomes unstable and a new distorted solution arises, which is stable. The formulation of the solution terms of elliptic integrals from (41) and (42) can also be helpful in asymptotic analysis of the solution. As k → 0, the complete elliptic integral of the first kind has the asymptotic behavior K (k ) = π 1 2 9 4 4 1 + k + k + o ( k ) . 2 4 64 (43) Therefore, we have an asymptotic expression for how φmax emerges from the uniform solution as φmax → 0+ in terms of the normalized field H / H c from 21 Hong Zhou, Eric P. Choate and Hongyun Wang 1 H 1 + φmax 2 + o (φmax 2 ) = 4 Hc (44) so that as φmax → 0+ φmax ≈ 2 As φmax → π 2 H −1 . Hc (45) , the asymptotic analysis gives (Stewart 2004): H 2 4 ≈ ln H c π 1 − sin 2 φmax (46) π H − 4 exp − . 2 2 Hc (47) which in turn yields φmax ≈ Thus, when φmax is close to The π 2 π when H H is big enough (for example, > 3 ). Hc Hc 1 dependence in these critical values corresponds with the dependence L found experimentally by Fredericks. Also, from an experimental point of view, they also provide a way to use the detection of the critical threshold to measure the Frank elasticity constants if the magnetic anisotropy χ a is known. 2.2 Bend and Splay Geometries A similar strategy may be followed in the bend and splay geometries, but each case depends on the two different Frank constants K1 and K 3 instead of just one. We will highlight the differences for the bend geometry, and the splay geometry can then be found by swapping the roles of K1 and K 3 . 22 Optical Fredericks Transition in a Liquid Crystal Layer Inserting the bend geometry form of n = ( sin φ ( z ) , 0, cos φ ( z ) ) and H = H (1, 0, 0 ) into (2) and (4), the total free energy density becomes = f 1 1 K1 sin 2 φ + K 3 cos 2 φ φ ′2 − χ a H 2 sin 2 φ . 2 2 (48) The Euler-Lagrange equation for the director angle (10) then becomes ( K sin 2 1 φ + K 3 cos 2 φ ) φ ′′ + ( K1 − K 3 ) sin 2φ 2 sin 2φ (49) φ ′ + χa H 2 0. = 2 2 Again, for any value of H and the boundary conditions (1), we have the uniform solution φ ( z ) = 0 . The second variation takes a similar form as (14) ∫ L 0 − χ a H 2η 2 + K 3η ′2 dz > 0 , (50) so that the uniform solution minimizes the free energy if H < H c where H c ,uniform = π L K3 χa . (51) For the distorted solution, we also assume the symmetry (17) and then solve integral equations first for φmax and then for φ ( z ) on 0 < z < L . Unfortunately, the 2 forms these integrals take are more complicated and cannot be easily represented with elliptic functions. We find these integrals by multiplying (49) by φ ′ and integrating with the same constant of integration as (20) so that ( K sin 1 2 φ + K 3 cos 2 φ ) φ ′2 = χ a H 2 sin 2 φmax − sin 2 φ . (52) Taking the square root and integrating, we can define the distorted solution with 23 Hong Zhou, Eric P. Choate and Hongyun Wang χ a Hz = ∫ φ 0 2 φ K + ( K − K ) sin φ K1 sin 2 φ + K 3 cos 2 φ 1 3 3 d φ = ∫ 0 sin 2 φmax − sin 2 φ dφ , sin 2 φmax − sin 2 φ (53) with φmax having been found from χa H 2 φmax K + ( K − K ) sin φ L 3 1 3 =∫ dφ . 0 2 sin 2 φmax − sin 2 φ (54) Or, using the change of variables (25), we have χ a Hz = ∫ sin φ sin −1 sin φmax 0 K 3 + ( K1 − K 3 ) sin 2 ψ sin 2 φmax dψ 1 − sin 2 ψ sin 2 φmax (55) π K 3 + ( K1 − K 3 ) sin 2 ψ sin 2 φmax L 2 χa H = ∫ dψ 0 2 1 − sin 2 ψ sin 2 φmax (56) We can find the critical field strength above which this distorted solution exists through a similar argument as the twist geometry by observing that the integrand in (55) and (56) is an increasing function of φmax so that K 3 + ( K1 − K 3 ) sin 2 ψ sin 2 φmax lim G (ψ , φmax ) = lim = φmax →0+ φmax →0+ 1 − sin 2 ψ sin 2 φmax K3 (57) Thus, taking the limit φmax → 0+ of (56) shows that χ a H c ,distorted L π K3 , = 2 2 (58) and again we have only one critical value H c ,bend = π L K3 χa , (59) which has the same dependence on the Frank constant as the twist (33) and single-constant approximations (40). A similar argument to the one above shows that 24 Optical Fredericks Transition in a Liquid Crystal Layer when H > H c ,bend , the distorted solution is energetically preferable to the uniform solution. The critical value for the splay geometry is H c , splay = π L K1 χa , (60) and the distorted solution is given by χ a Hz = ∫ χa H sin φ sin −1 sin φmax 0 K1 + ( K 3 − K1 ) sin 2 ψ sin 2 φmax dψ 1 − sin 2 ψ sin 2 φmax π K1 + ( K 3 − K1 ) sin 2 ψ sin 2 φmax L dψ . = ∫2 0 2 1 − sin 2 ψ sin 2 φmax (61) (62) 2.3 Extension to Electric Fields The above discussion of the Fredericks transition can be extended to include (1) pretilt at the boundaries where the boundary conditions φ= ( 0 ) φ= ( L ) 0 are replaced by φ= ( 0 ) φ= ( L ) φ0 ; (2) the tilted fields where the magnetic field is applied across the sample at a fixed angle; (3) weak anchoring where the director is weakly anchored to both boundary plates. A more detailed discussion can be found in Stewart (Stewart 2004) and Virga (Virga 1994). The Fredericks transition also occurs under the influence of an electric field E . From a mathematical perspective, the above analysis can be repeated with the magnetic free energy density (4) replaced by an electric free energy density 25 Hong Zhou, Eric P. Choate and Hongyun Wang 1 2 f electric = − ε a (n ⋅ E) , 2 (63) where ε a= ε − ε ⊥ is the dielectric anisotropy of the liquid crystal where ε and ε ⊥ are the relative permittivities or dielectric constants of the liquid crystal when the field and director are parallel and perpendicular, respectively. The analogous critical field strengths for the splay, twist and bend geometries are (Stewart 2004) = Ec , splay π K1 π K2 π = , Ec ,twist = , Ec ,bend L εa L εa L K3 εa . (64) However, this formulation is known to be less accurate than the magnetic field approximation. So far, we have assumed that the electromagnetic fields are unaffected by the orientation of the liquid crystal medium. For magnetic fields, this assumption works well, but for electric fields, the coupling of the field and the liquid crystal orientation cannot be ignored. 3. Optical Fredericks Transition with Coupled Orientation and Electromagnetic Fields We now extend our analysis in two ways to better model the optical Fredericks transition. That is, the reorientation of a nematic liquid crystalline cell by a light wave passing the layer allowing for the coupling of the electromagnetic field and the nematic orientation field. We use the bend geometry from Section 2 with the director n = (sin φ ( z ), 0, cos φ ( z )) , but the electromagnetic field consists of a normally incident beam of light with the polarization parallel to the xz-plane, as illustrated in Figure 4. In order to focus on the effect of the NLC, we assume the supporting plates have the same optical properties as the medium outside the cell, which we treat as vacuum. 26 Optical Fredericks Transition in a Liquid Crystal Layer 3.1 Maxwell Equations The governing equations of the electromagnetic field are given by Maxwell's equations (see, for example, Yeh 2005) which in Gaussian units are 1 ∂B =0 c ∂t (65) 1 ∂D 4π = J c ∂t c (66) ∇×E + ∇×H − ∇ ⋅ D = 4πρ (67) ∇ ⋅B =0 (68) for the electric field E , the magnetic field H , the electric displacement D , the magnetic induction B , and the speed of light c . We include the electric current density J and the charge density ρ for the moment, but we will soon assume they are zero. In order to close the system, it is necessary to specify constitutive relations that describe the macroscopic properties of the medium. The magnetic constitutive equation is B = µH , (69) where the relative permeability µ is assumed to be 1 so that the NLC has no effect on the magnetic field. The constitutive equation for the electric field is D= ε ⋅ E (70) for the symmetric relative permittivity tensor ε , which is also known as the dielectric tensor. If ε were a scalar, the system would be isotropic. Outside the NLC cell, we use ε = 1 . Inside the cell, the NLC is anisotropic with two different values of the relative permittivity. In the direction parallel to the director n , we have the extraordinary 27 Hong Zhou, Eric P. Choate and Hongyun Wang relative permittivity ε , but in the directions perpendicular to n , we have the ordinary relative permittivity ε ⊥ . Typical values for these constants for the nematic PAA at 125°C are ε ≈ 3.3 and ε ⊥ ≈ 2.3 . The relative permittivity tensor is ε ⊥ + ε a sin 2 φ 0 ε =ε ⊥ I + ε a nn = ε⊥ 0 ε a sin φ cos φ 0 ε a sin φ cos φ 0 ε ⊥ + ε a cos 2 φ (71) where I is the identity tensor and ε a= ε − ε ⊥ measures the dielectric anisotropy. Since these are linear equations, they apply to both real and complex electromagnetic vectors. However, since the real part of the product of two complex vectors is not equal to the product of their real parts, care must be taken to distinguish between the real and complex electromagnetic vectors in their products. The simplest form of light is a monochromatic, linearly polarized plane wave. So we assume a monochromatic complex form with angular frequency ω , and for the rest of this section, we use a tilde to denote the real, time-varying vectors. Vectors without tildes represent complex vectors that may depend on z but not t . That is, Re = E = ( Ee−iωt ) , D Re= ( De−iωt ) , H Re= ( He−iωt ) , B Re ( Be−iωt ) . (72) We can now use (69) and (70) to rewrite Faraday’s Law (65) and Ampere’s Law (66) as − iω ε ⋅ E = ∇ × H, c (73) iω (74) H = ∇ × E. c These allow us to condense the electromagnetic field equations into a single vector equation with E and n , which appears through ε , as 28 Optical Fredericks Transition in a Liquid Crystal Layer iω c ∇× ∇×E = − ε ⋅E c iω (75) or ∇ × (∇ × E) = ω2 c2 ε⋅E (76) which, with the help of the vector identity ∇ × ( ∇ × E ) = ∇ ( ∇ ⋅ E ) − ∇ 2 E , can be expressed as ∇ 2 E − ∇ ( ∇ ⋅ E ) + k0 2ε ⋅ E = 0 for the wavenumber k= 0 (77) ω 2π , where λ0 is the free space wavelength of the = c λ0 incident beam. This can be simplified further under our assumptions that the NLC and electromagnetic fields are homogeneous in both the x- and y-directions and the polarization of the incident beam has the electric field in the x-direction. From the z-component of (73), we observe that − ∂H 2 ∂H1 iω (ε13 E1 + ε 33 E3 ) = − =0 c ∂x ∂y (78) which implies that ε13 E1 + ε 33 E3 = 0 . This allows us to write the z-component of the electric field as a function of the x-component as ε ε sin φ cos φ E3 = − 13 E1 = − a E ε 33 ε ⊥ + ε a cos 2 φ 1 (79) A similar argument from (74) shows that H 3 = 0 . Also, the y-component of (73) is 29 Hong Zhou, Eric P. Choate and Hongyun Wang ∂ 2 E2 + k0 2ε ⊥ E2 = 0, 2 ∂z (80) and given the polarization of the incident beam, we can conclude that E2 = 0 . Furthermore, since ∂E ∂E ∂E iω H1 =3 − 2 = − 2 from (74), it follows that H1 = 0 . c ∂y ∂z ∂z Returning to (73), the x-component is d 2 E1 + k0 2 ( ε11 E1 + ε13 E3 ) = 0 2 dz (81) Substituting (79), this yields an equation connecting the x-component of the electric field and the director angle as ε ⊥ε || d 2 E1 + k0 2 E = 0. 2 ε ⊥ + ε a cos 2 φ 1 dz (82) Once E1 is known, we can find the y-component of the magnetic field from (74) to be H2 = 1 dE1 . ik0 dz (83) 3.2 Free Energy Minimization Now we need to minimize the free energy of the system to determine the preferred orientation of the system. The elastic free energy density f Frank is the same as (2). However, the electromagnetic contributions are more complicated due to the time-varying fields. The electric contribution is 1 1 Ee − iωt + E*eiωt ) ⋅ ( De − iωt + D*eiωt ) ⋅D = felectric = E ( 8π 32π 1 E ⋅ De − i 2ωt + E ⋅ D* + E* ⋅ D + E* ⋅ D*ei 2ωt ) = ( 32π 1 Re ( E ⋅ De − i 2ωt ) + E ⋅ D* = 16π (84) because E ⋅ D* is real. Similarly, we also have the magnetic contribution 30 Optical Fredericks Transition in a Liquid Crystal Layer 1 1 2 (85) B ⋅ H= Re ( B ⋅ He − i 2ωt ) + H . 8π 16π The time-varying Poynting vector, which represents the directional energy flux density fmagnetic= of the electromagnetic field, is c c Re ( E × He − i 2ωt ) + Re ( E × H* ) . E × H= 4π 8π The magnitude of the Poynting vector is the irradiance. S= (86) According to the energy conservation law Poynting’s theorem, the work done by the electric field is J= ⋅E 1 4π ∂D ⋅ E − + c∇ × H ∂t (87) with the insertion Ampere’s law (66). The first term can be written using the identity ∂ ∂E +E ⋅ ∂ D = ∂Ei ε E + E ε ∂E j = 2 ∂Ei ε E = 2E ⋅ ∂D ⋅D E⋅D = ij j i ij ij j ∂t ∂t ∂t ∂t ∂t ∂t ∂t ( ) (88) where we have used Einstein summation convention and the fact that ε is symmetric. ( ) ⋅∇ × H , ⋅∇ × E −E ×H = H The second term can be rewritten with the identity ∇ ⋅ E so that we can rewrite (87) as ( ) ( ( ) )) 1 ∂ − 2 ∂t E ⋅ D + c H ⋅∇ × E − ∇ ⋅ E × H 1 1 ∂ ˆ ∂B ×H = − c∇ ⋅ E E⋅ D − H⋅ − 4π 2 ∂t ∂t ∂ = − ( felectric + fmagnetic ) − ∇ ⋅ S . ∂t Under our assumption that the current density J is zero, then we have ⋅E J= 1 4π ( ( ) (89) ∂ (90) ( f electric + fmagnetic ) + ∇ ⋅ S = 0. ∂t For time-periodic sinusoidal electromagnetic fields, the average power flow per unit time is often more useful. We assume the timescale of the reorientation of the liquid crystal is much slower than the electromagnetic timescale defined by the frequency ω 31 Hong Zhou, Eric P. Choate and Hongyun Wang of our monochromatic incident beam. We therefore approach the liquid crystal part as a steady-state by averaging the appropriate electromagnetic quantities over one period. Therefore we need the time-average free energy densities over one period for the free energy minimization for the φ equation: 1 1 2 (91) f electric = felectric =E ⋅ D* , f magnetic = fmagnetic =H 16π 16π Also, to define the intensity below, we will also need the time-average of (90), or = 0 ∂ ( f electric + fmagnetic ) + ∇ ⋅ S ∂t ∂ ∂ c Re ( E × He − i 2ωt ) + Re ( E × H* ) (92) f electric + f magnetic + ∇ ⋅ ∂t ∂t 8π c = ∇⋅ Re ( E × H* ) = ∇ ⋅ S . 8π From the perspective of the free energy density of the orientation, the optical = energies are treated as negative quantities so that the free energy density is f = f Frank − f electric − f magnetic . (93) However, since f magnetic does not contain the director angle φ , its contribution to the free energy does not affect the minimization process, and so we omit it. We now proceed to minimize the free energy function in a manner similar to that of Section 2, except that it will contain the unknown E1 . The free energy density is f= (φ ( z ) , φ ′ ( z ) ) 2 1 K1 sin 2 φ ( z ) + K 3 cos 2 φ ( z ) φ ′ ( z ) 2 − E1 ( z ) 16π 2 ε ⊥ε (94) ε ⊥ + ε a cos 2 φ ( z ) Substituting this into the Euler-Lagrange equation (10), we find 32 Optical Fredericks Transition in a Liquid Crystal Layer 2 ( K1 sin φ + K3 cos φ ) ddzφ2 + ( K1 − K3 ) sin φ cos φ ddzφ (95) ε aε ⊥ε sin 2φ 2 E1 = + 0. 2 16π ( ε ⊥ + ε a cos 2 φ ) 2 2 2 3.3 Boundary Conditions and Intensity We now have a coupled second-order system (82) and (95) for the director angle φ and the x-component of the electric field E1 . We need boundary conditions for this system and a way to quantify the intensity of the electromagnetic field that will drive the optical Fredericks transition. For the anchoring conditions, we use φ ( 0 ) = 0, φ ( L) = 0. (96) The electromagnetic boundary conditions are more complicated. When the middle layer ( 0 < z < L ) is homogeneous and isotropic, boundary conditions have been given in (Yeh 2005). In our study here, the middle layer is an NLC so we cannot directly use the boundary conditions in (Yeh 2005). However, we can borrow ideas from there. Outside the liquid crystal layer, E1 is assumed to take the forms Ein eik0 z + Eref e − ik0 z , z < 0 E1 ( z ) = Eout eik0 z , z>L (97) where the unknown complex constants Ein , Eref , and Eout represent, respectively, the incident beam, the beam that reflects off the front of the NLC cell, and the transmitted beam that passes through the cell. From (83), the corresponding magnetic field outside the layer is 33 Hong Zhou, Eric P. Choate and Hongyun Wang E eik0 z − Eref e − ik0 z , z < 0 H 2 ( z ) = in Eout eik0 z , z>L (98) Ideally, we would like to impose Ein and then solve for Eref and Eout . However, it is not possible to do this since it would not assign a boundary condition to the system (82) and (95). We can get this around in the following way. From the time-average Poynting vector (92), it follows that d c d Re ( E1 H 2* ) 0 . = S3 = 8π dz dz Thus, S3 = (99) c Re ( E1 H 2* ) is constant throughout the domain, both inside and 8π outside the NLC cell. Note that it is only the time-average of the z-component of the Poynting vector that is constant throughout the domain, not the overall Poynting vector, its magnitude, or S3 itself. We define the intensity I as this constant so that ( 2 c E − Eref in 8π c * I = = Re ( E1 H 2 ) c 8π 2 Eout , 8π 2 2 ), z<0 (100) z>L Thus, we can conclude that = Ein Eref + Eout , as is required to conserve energy. 2 We shall choose Eout = 2 8π I but choose I as our control variable. c For discontinuous media, the components of the electromagnetic fields that are tangential to the surfaces of the discontinuities must be continuous. For our NLC cell, this means that E1 and H 2 must be continuous at both z = 0 and z = L . This gives us both boundary conditions for (82) and way to solve for the unknowns Ein and Eref . For E1 , we have 34 Optical Fredericks Transition in a Liquid Crystal Layer Ein + Eref = E1 ( z = 0 ) (101) Eout = eik0 L E= L) 1(z For H 2 , (83) gives us 1 dE1 Ein − Eref =H 2 ( z =0 ) = ik0 dz 1 dE1 Eout e = H 2 (= z L= ) ik0 dz ik0 L z =0 (102) z=L Since (82) is linear in E1 , we use the rescaling E1 ( z ) = Eout eik0 L u ( z ) E1 ( z ) = 2 2 8π I u ( z) c (103) so that our solution proceeds as follows. For a given for a given intensity I , we first define Eout = 8π I . Then we solve c ε ⊥ε || d 2u 0, u= + k0 2 2 dz ε ⊥ + ε a cos 2 φ 2 (104) ( K1 sin φ + K3 cos φ ) ddzφ2 + 12 ( K1 − K3 ) sin 2φ ddzφ I ε aε ⊥ε sin 2φ 2 0, u = + 2 2c ( ε ⊥ + ε a cos 2 φ ) 2 2 2 subject to the four boundary conditions φ ( 0 ) = 0, du dz φ ( L) = 0, u ( L ) 1,= ik0 . = z=L (105) Then, we may write 35 Hong Zhou, Eric P. Choate and Hongyun Wang , 1 1 du = Eref Eout eik0 L u ( 0 ) − z =0 . ik0 dz 2 As in Section 2, for any value of I, we have the solution with the uniform = Ein 1 1 du Eout eik0 L u ( 0 ) + ik0 dz 2 z =0 (106) orientation φ ( z ) = 0 . The corresponding electric field is the same as the case of an isotropic layer with permittivity ε ⊥ . This solution is only stable for values of I less than some critical intensity I 2 . There is a second nonuniform solution that only exists for a values of I greater than a critical intensity I1 . Unlike the problem in Section 2, these critical values are not the same, and we have hysteresis with two stable solutions in the region I1 < I < I 2 . 4. Numerical Method and Results We approximate the orientation angle profile φ ( z ) using a truncated Fourier sine expansion: z K kπ z φ ( z ) =φ0 + (φL − φ0 ) + ∑ wk sin L k =1 L (107) In this formulation, the orientation angle profile is represented by a vector of K components w = w1 , w2 , , wK . As a result, the free energy is a function of the vector w. L To calculate the free energy F ( w ) defined as F [fff ] = ∫ f ( ( z ) , ′ ( z ) )dz with 0 the free energy density f (ff ( z ) , ′ ( z ) ) given in (94), we first calculate functions φ ( z ) and φ ′ ( z ) from vector w = w1 , w2 , , wK on a fine numerical grid. Next, u ( z ) is solved from (104) and (105) on the same numerical grid using the fourth order Runge-Kutta method. The free energy density f (φ ( z ) , φ ′ ( z ) ) is 36 Optical Fredericks Transition in a Liquid Crystal Layer evaluated on the numerical grid from functions φ ( z ) , φ ′ ( z ) and u ( z ) . Finally, the free energy F ( w ) is calculated by integrating the free energy density f (φ ( z ) , φ ′ ( z ) ) given in (94) on the numerical grid. Once we have a numerical method for calculating F ( w ) at each value of beam intensity I and for each coefficient vector w , we solve numerically ∇F ( w ) = 0 for steady states. The stability of each steady state is determined by examining whether or not the Hessian matrix H ( F )( w ) is positive definite. In numerical simulations, both the gradient ∇F ( w ) and the Hessian matrix H ( F )( w ) are calculated using numerical differentiation. The problem is specified by parameters below. • the anchoring conditions at the two boundaries, φ0 , φL • the ordinary relative permittivity, ε ⊥ = 2.45 • the extraordinary relative permittivity, ε = 3.346 • two Frank elasticity constants, K= 9.5 ×10−7 dyn 4.5 ×10−7 dyn , K= 3 1 • thickness of the layer, L = 200 nm • wavelength of the beam, λ0 = 1.5μm • light speed, c= 3 ×1010 cm/s • 2 I 0.1 0.7 GW/cm 0.1 0.7 ×1016 dyn/ ( cm s ) = = intensity of the beam, The derived parameters are • ε a= ε − ε ⊥ • k0 = 2π λ0 wavenumber of the beam 37 Hong Zhou, Eric P. Choate and Hongyun Wang • E out = 8π I c Below we study the steady states and their stabilities as a function of the beam intensity I. We first consider the simplest anchoring conditions: φ= φ= 0 . For this anchoring 0 L condition,= φ ( z ) 0= i.e. w 0 is always a steady state solution (trivial branch) for any ( ) beam intensity I. Another branch of steady state solution appears at I = 0.210578 and is stable. The trivial branch w = 0 remains stable beyond I = 0.210578 ; it becomes ( ) unstable at I = 0.214293 . The phase diagram is shown in Figure 5. In the figure, the vertical coordinate is the maximum orientation angle: max φ ( z ) / (π / 2 ) . There is a z small interval for the beam intensity I in which both the trivial branch and the non-trivial branch are stable. The system has a hysteresis behavior: when the beam intensity is increased from a low value the transition from the trivial branch to the non-trivial branch occurs at I = 0.214293 ; when the beam intensity is reduced from a high value the transition from the non-trivial branch to the trivial branch occurs at I = 0.210578 . Figure 6 shows the details of the phase diagram in the small interval for the beam intensity I where both trivial branch and the non-trivial branch are stable. 5. Conclusion and Future Perspective The Fredericks transition plays an important role in nonlinear optics and it can occur under magnetic or electric effects. Even though it has been studied extensively both experimentally and theoretically, there are still many problems that remain to be solved. For example, a rigorous mathematical proof on the hysteresis of the Fredericks transition is still unavailable; the transition for the mismatched boundary conditions 38 Optical Fredericks Transition in a Liquid Crystal Layer needs further investigation. To conclude, Fredericks transition will continue to be an active research subject. Acknowledgment and Disclaimer Hong Zhou would like to thank the Office of Naval Research (ONR) for supporting this work. The views expressed in this document are those of the authors and do not reflect the official policy or position of the Department of Defense or the U.S. Government. References Bena R, Petrescu E (2003) Surface effects on magnetic Freedericksz transition in ferronematics with soft particle anchoring. Journal of Magnetism and Magnetic Materials 263:353-359 Burylov SV, Raihker YL (1993) Magnetic Fredericksz transition in a ferronematic. Journal of Magnetism and Magnetic Materials 122:62-65. Chandrasekhar S (1992) Liquid Crystals. Cambridge University Press, Cambridge. Durbin SD, Arakelian SM, Shen YR (1981) Optical-field-induced birefrigence and Freedericksz transition in a nematic liquid crystal. Physical Review Letters 47(19): 1411-1414 39 Hong Zhou, Eric P. Choate and Hongyun Wang de Gennes PG and Prost J (1993) The Physics of Liquid Crystals. Clarendon Press, Oxford. de Jeu WH (1980) Physical Properties of Liquid Crystalline Materials. Gordon and Breach, New York. Deuling HJ, Helfrich W (1974) Hysteresis in the deformation of nematic liquid crystal layers with homeotropic orientation. Applied Physics Letters 25: 129-130 Freedericksz V, Zolina V (1933) Forces causing the orientation of an anisotropic liquid. Transactions of the Faraday Society 29:919-930 Ilyina V, Cox SJ and Sluckin TJ (2006) A computational approach to the optical Freedericksz. Optics Communications 260: 474-480 Khoo IC (1981) Optically induced molecular reorientation and third-order nonlinear optical processes in nematic liquid crystals. Physical Review A 23(4): 2077-2081 Khoo IC (1982a) Nonlinear light scattering by laser- and dc-field-induced molecular reorientations in nematic-liquid-crystal films. Physical Review A 25(2): 1040-1048 Khoo IC (1982b) Theory of optically induced molecular reorientations and 40 Optical Fredericks Transition in a Liquid Crystal Layer quantitative experiments on wave mixing and the self-focusing of light. Physical Review A 25(3): 1636-1644 Khoo IC, Zhuang S (1980) Nonlinear optical amplification in a nematic liquid crystal above the Frederiks transition. Applied Physics Letters 37: 3-4 Khoo IC (1995) Liquid Crystals: Physical Properties and Nonlinear Optical Phenomena. Wiley, New York. Li F, Buchnev O, Cheon C, Glushchenko A, Reshetnyak V, Reznikov Y, Sluckin TJ, West JL (2006) Orientational coupling amplification in ferroelectric nematic colloids. Physical Review Letters 97:147801 Miroshnichenko AE, Pinkevych I, Kivshar YS (2006) Tunable all-optical switching in periodic structures with liquid-crystal defects. Optics Express 14(7): 2839-2844 Ong HL (1983) Optically induced Freedericksz transition and bistability in a nematic liquid crystal. Physical Review A 28(4): 2393-2407 Petrescu E, Bena E (2009) Surface anchoring energy and the Freedericksz transitions in ferronematics. Journal of Magnetism and Magnetic Materials 321: 2757-2762 41 Hong Zhou, Eric P. Choate and Hongyun Wang Rapini A, Papoular M (1969) Distortion d’une lamelle nematique sous champ magnetique conditions d’ancrage aux parois. J de Phys. Colloq. 30:C4-54-C4-56. Reznikov Y, Buchnev O, Tereshchenko O, Reshetnyak V, Glushchenko A, West J (2003) Ferroelectric nematic suspension. Applied Physics Letters 82(12):1917-1919 Self RH, Please EP, Sluckin TJ (2002) Deformation of nematic liquid crystals in an electric field. European Journal of Applied Mathematics 13:1-23 Shelestiuk SM, Reshetnyak V, Sluckin T (2011) Frederiks transition in ferroelectric liquid-crystal nanosuspensions. Physical Review E 83: 041705 Shi J (2002) Criteria for the first order Freedericksz transitions. Liquid Crystals 29(1):121-125 Shi J, Yue H (2000) Surface- and optical-field-induced Freedericksz transitions and hysteresis in a nematic cell. Physical Review E 62(1):689-698 Shoarinejad S, Shahzamanian MA (2008) On the numerical study of Frederick transition in nematic liquid crystals. Journal of Molecular Liquids 138: 14-19 Stark H (2001) Physics of colloidal dispersions in nematic liquid crystals. Physics 42 Optical Fredericks Transition in a Liquid Crystal Layer Reports 351: 387-474 Stewart IW (2004) The Static and Dynamic Continuum Theory of Liquid Crystals: A Mathematical Introduction. Taylor & Francis, London Sugimura A, Luckhurst GR, Ou-Yang Z (1995) Director deformation of a twisted chiral nematic liquid crystal cell with weak anchoring boundaries. Physical Review E 52(1):681-689 Torrent MC, Sagues F, Arias F, San Miguel M (1988) Freedericksz transition in a periodic magnetic field. Physical Review A 38(5): 2641-2649 Vena C, Versace C, Strangi G, D'Elia S, Bartolino R (2007) Light depolarization effects during the Freedericksz transition in nematic lquid crystals. Optics Express 15(25): 17063-17071 Virga EG (1994) Variational Theories for Liquid Crystals. Chapman and Hall, London. Yang G, Shi J, Liang Y (2000) Surface anchoring energy and the first order Freedericksz transition of a NLC cell. Liquid Crystals 27(7):875-882 43 Hong Zhou, Eric P. Choate and Hongyun Wang Yang KH (1983) Freedericksz transition of twisted nematic cells. Applied Physics Letters 43: 171-173 Yeh P (2005) Optical Waves in Layered Media. Wiley, Hoboken, New Jersey Yilmaz S, Melik H, Angay F, Emek M, Yildirim A (2008) Optical properties of aligned nematic liquid crystals in electric field. Journal of Modern Physics 2: 248-255 Zakhlevnykh AN (2004) Threshold magnetic fields and Freedericksz transition in a ferronematic. Journal of Magnetism and Magnetic Materials 269:238-244 Zel’dovich BY, Tabiryan NV (1980) Light self-focussing in nematic liquid crystals as a method of investigation of the free surface orienting influence. Sov. Phys. JETP 52 :1210 Zel’dovich BY, Tabiryan NV, Chilingaryan, YS (1981) Fredericks transitions induced by light fields. Sov. Phys. JETP 54(1):32-37 Zocher H (1933) The effect of a magnetic field on the nematic state. Transactions of the Faraday Society 29:945-957 44 Optical Fredericks Transition in a Liquid Crystal Layer Figure 1: An illustration of the three common geometries. 45 Hong Zhou, Eric P. Choate and Hongyun Wang Figure 2: The solution φ ( z ) with respect to π / 2 for different values of dimensionless magnetic field strength H / H c using the one-constant approximation. 46 Optical Fredericks Transition in a Liquid Crystal Layer Figure 3: Phase diagram of the classical Fredericks transition in the one-constant approximation. 47 Hong Zhou, Eric P. Choate and Hongyun Wang (a) (b) Figure 4: A schematic diagram of an incident beam on a nematic liquid crystal layer. 48 Optical Fredericks Transition in a Liquid Crystal Layer Figure 5: Phase diagram for the anchoring condition φ= φ= 0. 0 L = φ ( z ) 0= i.e. w 0 is always a steady state solution. A second branch of steady ( ) solution appears at I = 0.210578 and is stable. The trivial branch w = 0 ( ) remains stable beyond I = 0.210578 ; it becomes unstable at I = 0.214293 . 49 Hong Zhou, Eric P. Choate and Hongyun Wang Figure 6: Details of the phase diagram in the small interval where both the trivial branch and the non-trivial branch are stable. 50